Label-free electrochemical biosensor based on green-synthesized reduced graphene oxide/Fe3O4/nafion/polyaniline for ultrasensitive detection of SKBR3 cell line of HER2 breast cancer biomarker

Cancer stands as one of the most impactful illnesses in the modern world, primarily owing to its lethal consequences. The fundamental concern in this context likely stems from delayed diagnoses in patients. Hence, detecting various forms of cancer is imperative. A formidable challenge in cancer research has been the diagnosis and treatment of this disease. Early cancer diagnosis is crucial, as it significantly influences subsequent therapeutic steps. Despite substantial scientific efforts, accurately and swiftly diagnosing cancer remains a formidable challenge. It is well known that the field of cancer diagnosis has effectively included electrochemical approaches. Combining the remarkable selectivity of biosensing components—such as aptamers, antibodies, or nucleic acids—with electrochemical sensor systems has shown positive outcomes. In this study, we adapt a novel electrochemical biosensor for cancer detection. This biosensor, based on a glassy carbon electrode, incorporates a nanocomposite of reduced graphene oxide/Fe3O4/Nafion/polyaniline. We elucidated the modification process using SEM, TEM, FTIR, RAMAN, VSM, and electrochemical methods. To optimize the experimental conditions and monitor the immobilization processes, electrochemical techniques such as CV, EIS, and SWV were employed. The calibration graph has a linear range of 102–106 cells mL−1, with a detection limit of 5 cells mL−1.


Methods and apparatus
The morphology characteristics of the nanocomposite were analyzed using transmission electron microscopy (FEI Tecnai F20 series) and scanning electron microscope (AIS 2100, Seron Technologies, Korea) with 5000, 10,000, and 30,000 magnifications.For the ultrasonic irradiation, a PARSONIC 15S ultrasonic bath operating at a frequency of 28 kHz was employed.Every electrochemical experiment was conducted using an Autolab PGSTAT 30 (Echo Chemie, B. V., Netherlands) equipped with a three-electrode apparatus: a modified GCE as the working electrode, Ag/AgCl as the reference electrode, and Pt rod as the counter electrode.To create error bars, each electrode was examined 3 times for each experiment.

Synthesis of nanocomposite
The process diagram for the creation and functionalization of nano-biosensors employing the sandwich rGO/ Fe 3 O 4 /Nafion/PANI for the detection of SK-BR3 is shown in Fig. 1.

Graphene oxide synthesis
According to the literature, a modified Hummer was used to generate the GO using graphite fine powder, H 2 SO 4 , H 3 PO 4 , and KMnO 4 .In summary, at 75 °C, a mixture of phosphoric acid, sulfuric acid (40:360 mL), graphite and potassium permanganate (3:18 g) was first formed.After being shaken and stirred for 12 h, the two solutions were cooled to 25 °C and placed in an ice bath with 6 mL of 30% hydrogen peroxide added.Following centrifugation, the final product underwent purification.The resultant dilution was centrifuged, filtered, and washed with a 1:10 chlorhydrate (30% v/v, 250 mL) to remove any remaining ions.The filter was then reused.Before being cleaned with a 200 mL EtOH solution.

Preparation of Fe 3 O 4 -rGO nanomaterials
Green synthesizing rGO Using 0.1 M AA and 50 mL of GO solution (0.1 mg mL −1 ), a volume ratio of 1:1 was obtained on a heating plate 41 .Following that, the mixture was swirled for 30 min while being heated to 70 °C.The solution's hue shifted from brownish-yellow to black throughout this period.The residual solid (i.e.rGO) was what remained after the product was centrifuged three times with ethanol and water to remove the supernatant.After that, it was baked to dryness at 120 °C.

Anchoring Fe 3 O 4 on rGO
Generally, ultrasonication was used to disperse 500 mg of rGO in distilled water for 2 h.Following the addition of FeSO 4 •7H 2 O (0.002 mol) and FeCl 3 •6H 2 O (0.004 mol), the mixture was ultrasonicated for an hour.About 1.65 mM NH 4 OH solution was dropped and continuously spun for 2 h.Once the resultant black substance was filtered and repeatedly washed with water to remove any residual acid and dissociative Fe(II), it was treated with ethanol.After immersing the solid for 60 min in anhydrous ethanol, then filtered and vacuum-dried at 100 °C42,43 .

Optimization of Nafion percentages in the rGO-Fe 3 O 4 -Nafion composite
To improve an electrochemical sensor's sensitivity (specific experimental parameters), the ratio of Nafion to Fe 3 O 4 -Nafion in rGO was tuned.By utilizing a CCD and the RSM, we evaluated the impacts of the Nafion concentration ratio and the length of the incubation period.Consequently, Table 2 displays the outcomes of a two-factor and three-level fractional factorial CCD design.The trial's statistical design was created using the Design-Expert 11 tool.We looked at the effects of Nafion percentage in composites ranging from 0.05 to 0.1% w/w and incubation time between 30 and 60 min.Design of experiment (DoE) evaluated the effects of two factors on current: Nafion percentages and incubation time.Table 1 displays the range of these characteristics that apply.In order to maximize the current, a factorial design was taken into consideration, and Table 2 displays the runs under various circumstances.

Modification of GCE and preparation of GCE sensor
Following a thorough polishing process utilizing aluminum oxide 0.05, 0.3, and 1.0 µM powders in that sequence, and a thorough washing in ethanol and water solution between polishing steps, it was ultrasonicated for 5 min, followed by pure water, before being dried with N 2 gas. 10 µL of the rGO-Fe 3 O 4 -Nafion suspension were poured onto the GCE's surface in the second stage, and it was allowed to air dry.The PANI layer on the electrode surface was then electropolymerized using a solution of 0.2 M aniline and 0.5 M H 2 SO 4 .
As a consequence, the potential range was altered to − 0.15 to 1.2 V and the scan rate was increased to 20 mV s −1 for 10 cycles 44 .Microscopic methods like TEM and SEM were employed to verify that the produced nanocomposite and coated electrode met all specifications and was of superior quality.To activate carboxylic groups, the designed electrode was maintained in the (NHS/EDC) dissolution (1.0 mM) for 60 min at room temperature after the rGO-Fe 3 O 4 -Nafion/PANI/GCE was washed with double deionized water (DDW) in the fourth stage.In a wet chamber, 10 µL of a 1 mg mL −1 herceptin solution were dropped over the electrode surface for a duration of 12 h, constituting the fifth step.This electrode was designated as rGO-Fe 3 O 4 -Nafion/PANI/ GCE.Then, in order to cover any exposed target surface regions that were still uncoated with biomolecules and eliminate nonspecific binding, the rGO-Fe 3 O 4 -Nafion/PANI/GCE electrode was submerged in a 0.1% BSA solution for 40 min.Table 1.Variables chosen for the experiment's design, as well as their significance levels.

Morphology characterization
On the GC, the prepared material was placed and the electrodes were cleaned accordingly.After that, biosensing selectivity, calibration, and activity tests were utilized.The FTIR spectroscopy of produced materials was assessed to examine the functional groups present in rGO-Fe 3 O 4 (Fig. 4).Raman spectroscopy is an effective technique for determination of the composition and structural characteristics of materials.Raman spectroscopy was used to investigate the samples in order to determine their structural characteristics (Fig. 5).The VSM test (Fig. 6) was utilized to identify the type of magnetization produced by an applied external magnetic field.SEM was used to evaluate the surface morphologies of GO (Fig. 2a), rGO (Fig. 2b), rGO-Fe 3 O 4 (Fig. 2c), and rGO-Fe 3 O 4 -nafion/PANI (Fig. 2d).From a petal-like angle, the SEM of GO in Fig. 2a depicts the porous graphene nanosheets that resemble nests.Following the reduction procedure, the GO folded sheets showed an exfoliated sheet-like shape and were well reduced, resulting in a greater surface area (Fig. 2b).There are some exfoliated layers and nest-like porosity on the surface of the PANI/GO/GCE electrode, as shown in Fig. 2d.The PANI/GCE coarser's SEM also shows some exfoliated layers.When acid is added to aniline oligomers or aniline amines, a nanowire-shaped PANI is formed, as shown in Fig. 2d.

FTIR
In Fig. 4, the FTIR spectra of the composites GO, rGO, PANI, and rGO-PANI are shown.The nanocomposite's characteristic FTIR spectrum agrees with earlier research.The characteristic peaks of the GO spectra were formed by C-H stretching, C=C stretching, C-H bending, C-O stretching, and OH out-of-plane bend at 3060.22, 1643.39,1433.05,1091.47, and 599.28 cm −1 , respectively.These peaks were absent from the graphite spectra, indicating that significant oxygen-containing functional groups were added to GO by the oxidation processes 45 .
The rGO peaks, which are 3060.22,1643.39,1433.05,1091.47, and 599.28 cm −1 , all showed a substantial drop when compared to the GO peak, providing additional strong evidence of reduction.All rGOs exhibit a reduction in the strength of these GO peaks, which suggests a certain degree of elimination of functional groups that contain oxygen 46 .
These functional groups are also present in GO-Fe 3 O 4 , but they are red-shifted in the bond locations and have altered peak sharpness, especially in the case of aromatic C=C bonding.This suggests that different functional groups in GO-Fe 3 O 4 are operating in a different coordinating context.The peaks in the 400-700 cm −1 range correlate to the Fe-O content of Fe 3 O 4 .The suggestion is that covalent bonding in GO is supported by the change in C=C bonding and peak position shift.The decrease of GO is shown by the lower absorbance intensity of several functional groups in rGO-Fe 3 O 4 as compared to GO-Fe 3 O 4 47 .www.nature.com/scientificreports/New peaks were also observed for the C=N (1571 cm −1 ), C-N (1237 cm −1 ), C-H stretching vibration (873 cm −1 ), and C=C of the quinoid and benzenoid rings (1486 and 1300 cm −1 ) of PANI.The successful integration of PANI was confirmed by these outcomes 48 .

RAMAN
Raman spectroscopy is the most efficient technique for characterizing carbon-based materials.The Raman spectra of GO, rGO, rGO-Fe 3 O 4 , and rGO-Fe 3 O 4 -Nafion/PANI nanocomposites are shown in Fig. 5.The breathing mode of j-point photons with A1g symmetry produces the D vibration band, which may be seen at 1364 and 1354 cm −1 .Figure 5 shows that it is 20 cm −1 for rGO and GO, respectively.On the other hand, the G vibration band was found to be produced at 1594 cm −1 for GO and 1600 cm −1 for rGO by first-order E2g phonon scattering from sp 2 carbon.All sp 2 carbon systems have a stretching C-C bond, which also affects the G vibration band.The disorder bands and tangential bands are represented, respectively, by the Raman spectra's D and G bands.
It was found that GO has an I D /I G ratio of 0.855.Because the sp 2 carbon was restored after reduction, the average sizes of the sp 2 domains decreased while the ID/IG for rGO rose.The greater intensity in the D band was another clue that rGO included more isolated graphene domains than GO; this difference might have been caused by the O 2 moiety in GO being removed during reduction.It was discovered that GO's ID/IG ratio was 0.855.The average sizes of sp 2 domains shrank and the I D /I G for rGO increased upon restoration of sp 2 carbon following reduction.The greater intensity in the D band, which was most likely brought on by the removal of GO's oxygen moiety during reduction, provided additional proof that rGO contained more isolated graphene domains than GO 49 .
The peaks that appeared in the ternary composite's Raman spectrum reveal PANI chains that developed on the surface of the rGO/Fe 3 O 4 composite.These peaks combine the bonds seen in the PANI and rGO/Fe 3 O 4 samples.Because of the π-π interaction between PANI and rGO, the G band blue-shifts in the Raman spectra of rGO/Fe 3 O 4 /PANI while the D band remains unchanged 50,51 .It was indicated that PANI had been added to the composites by the existence of peaks in the rGO/Fe 3 O 4 /PANI spectrum.The C-C stretching (1397 cm −1 ), C=C (1483 cm −1 ), and in-plane C-H bending of the benzenoid ring (1250 cm −1 ) of the quinoid ring were all correlated with these peaks.

Magnetic properties
In the magnetic field range of − 8000 to + 8000 Oe, the M-H curves of the room-temperature rGO/Fe 3 O 4 and rGO/Fe 3 O 4 /PANI composites are displayed in Fig. 6.The VSM investigations of the GO and rGO (nanocomposite) show that both graphs have very low magnetic remanence.This suggests that when the external magnetic field is removed, the magnetic property disappears 52

Electrochemical characteristics
The Nyquist plot and CV are clearly understood, as shown in Figs.7 and 8, with the peak height of the CV lowering when the electrode was functionalized using rGO-Fe 3 O 4 -Nafion/PANI/GCE.The rGO-Fe 3 O 4 -Nafion/ PANI and glassy carbon electrode's effective charge mediation may be the reason why the redox peaks of the rGO-Fe 3 O 4 -Nafion/PANI/GCE with cells were lower than those of the bare electrode.One method used in electrochemical characterization is impedance spectroscopy.Nevertheless, the impedance approach is only partially quantitatively applied for biosensing assessment and detection.Moreover, interferences may affect the results and reduce selectivity as this method uses resistance to the analyte's detection.

CV
After the electrode was modified with a nanocomposite, BSA, and cancer cell in a Fe(CN) 6 3−/4− probe, CV was achieved to evaluate electrochemically the surface change of the electrode (Fig. 7).For bare GCE, a very low background current was seen (Fig. 7a).Nevertheless, when standard rGO/Fe 3 O 4 -Nafion was adapted onto the electrode, two oxidation and reduction peaks were seen, and the voltammetric signal rose.Figure 7c shows that the reversible electron transfer process benefited from the presence of rGO/Fe 3 O 4 -Nafion.Comparatively speaking, the modified electrode increased the effective surface area, raised the electron transfer rate, and raised the electrochemical activity.Peak current is likely higher because of rGO's special qualities, which include large surface area, fast electric transfer rates, and superior conductivity.Moreover, using Fe 3 O 4 nanoparticles can boost the electrode's accessible surface area.
The inset of Fig. 7 illustrates how the peak current rises and how the CV response of rGO/Fe 3 O 4 -Nafion is notably lower than the CV response.An enhancement in the electrode's conductivity, a reduction in the absence of PANI, and an increase in the active surface area all contribute to these outcomes.Stated differently, the PANI electrodeposition led to an increase in the cover's electrode performance and activity.As anticipated, Herceptin immobilization results in a sharp drop in current, which is further diminished when cancer cells are added.These results show that the addition of Herceptin to the surface electrode was successful.Throughout the building process, the surface changes were tracked using the CV.Following the application of the rGO/Fe 3 O 4 -Nafion-PANI nanocomposite to the GCE, the bare GCE's R ct was significantly reduced.The resistance drops greatly increased the electrode's sensitivity and detection limit.Due to the non-electroactive biomolecule of the antibody, which blocked the surface and impeded charge transfer after it was deposited, the antibody's attachment to the nanocomposite's surface greatly reduced the R ct .The R ct increased when BSA was introduced after that.The incubation time resulted in specific adsorption between the antibody and antigen, which preferentially adhered the cancer cells to the functionalized electrode and significantly raised R ct .

Optimization of the Herceptin concentration and incubation times
The Herceptin concentration was further adjusted for several probe concentrations of 1 × 10 -8 , 2 × 10 -8 , 5 × 10 -8 , and 1 × 10 -7 M. To enhance this characteristic, several incubation times, including 30, 40, 60, and 120 min, were explored.The findings show that the ideal duration of contact is around 30 min, during which time all necessary incubation is finished.To enhance the biosensor's detecting capabilities, it is imperative to augment the biomolecule's immobilization amount.

Optimization of temperature and pH
The electrolyte's temperature affects the electrochemical reaction.Consequently, the nano-performance biosensor was evaluated across a range of temperatures (30, 35, 45, 55, and 65 °C).Because biomolecules are heatsensitive by nature, it was shown that 35 °C, or almost human physiological temperature, was the ideal working temperature for biomolecule detection in Fe(CN) 6 3−/4− solution (Fig. 9).Not to mention, the pH level needs to be changed.Biomolecules can break down into their parts, such as sugar, bases, and phosphate, in an extremely acidic incubation medium, but they can also be disturbed in a somewhat acidic environment.Hydrogen bonds maintain the interaction between the antigen and the antibody.Furthermore, the hydrogen bonds between antibody pairs may cause the antigen's structure to be disturbed.To investigate how pH affected the biosensors' stability, a variety of pH-varying electrolytes were found (Fig. 10).It has been demonstrated that a pH of 7.4 produces the best biosensing system.After adjusting the functionalization settings, the best values-including sensor calibration-are chosen for the biosensing study.

Experimental design
The data was analyzed using five different models: mean, linear, 2FI, quadratic, and cubic.The quadratic model was selected due to its highest-order polynomial and substantial sum of squares.The response surface quadratic    www.nature.com/scientificreports/model's Analysis of Variant (ANOVA) was used to determine the parameters influencing cell growth and the fitted model's significant level.The quadratic model's ANOVA is displayed in Table 3.The F and p values show the intensity of the interaction between each independent variable and the importance of each coefficient.The model is significant if the value of "Prob > F" is less than 0.005, and vice versa.Table 3 indicates that the model's p-value was less than 0.001, and its F-value was high, suggesting that the model was important in explaining the data.This suggested that the model provided the necessary signals for navigating the design space.An excellent indicator was the R 2 value of 0.9710, which demonstrated that a significant amount of variability-up to 98%-was explained by the data.
All two of the parameters had a statistically significant favorable influence on the development of electrical current, according to the ANOVA analysis.The coefficients found in the final equation, according to Anderson and Whitcomb, may be directly compared to determine the relative importance of the various elements.Figure 11 utilizes a bar graph to demonstrate the relative influence of the influencing elements.This figure demonstrated how each factor's influence on each response changed, leading to the conclusion that agitation speed had the most effect on current.
Consequently, a quadratic polynomial equation was used to regress the experimental results derived from the CCD.The resulting regression equation is displayed below, with the actual elements being represented.
Using software designed to maximize current at a single ideal state, a numerical optimization process produced all the optimum circumstances.The optimum response was validated using a nafion concentration of 0.081% and an incubation duration of 49.77 min.The following graphic illustrates, in three dimensions, how the two critical factors-nafion % and incubation time-affect the reaction to the flow differential.In the accompanying image, the Design Expert program offers the ideal circumstances.
Figure 12 compares the actual and expected values.It was successful in bridging the association between process variables and the current that the projected values achieved.

Selectivity analysis
The most crucial components of a biosensor's sensing ability are its selectivity and responsiveness in real biospecimens containing electroactive chemicals.For this investigation, we used a range of cell lines, including the human normal liver cell line, MCF-7, and SK-BR-3.At each step, 100 cells mL −1 of cell solution were dropcoated.SWV analysis was performed prior to and after insertion of the cells onto the electrode surface in each case.We determine the parameter ΔI/I by dividing the intensity difference between SWV peaks on the main intensity (prior to cell implantation) in order to exclude the electrode difference parameter from the selectivity findings.Figures 13 and 14 display the whole data comparison together with the pertinent curves.Compared to the findings for the other cell lines, SK-BR-3 cells appear to have a ΔI/I ratio greater than 0.34.This suggests that in SK-BR-3 cells, the number of cells linked to electrodes was greater than that of other cells, indicating the exceptional affinity and selectivity of Herceptin antibodies for the HER2 receptors.Figure 13  The linear range of biosensor typically indicates the range of analyte concentrations for which it displays an acceptable linear corresponding response.To accomplish the linear dynamic range of immunosensor for detecting HER2 + over-expression on the SK-BR3, an updated electrochemical cell and rGO-Fe 3 O 4 -Nafion/ PANI electrode were utilized.By adding SK-BR-3 to the electrode surface in varying quantities, the biosensor's linear range was determined.After that, the SWV graphs were compared, leading to the following deductions.
We found that for 4 out of 6 tests, the ΔI/I was greater than 0.34.We also tested the practicality and durability of the synthetic material for 2 weeks.So, not only the hybrid material could be made quickly and cost-effectively, but this biosensor could also be used to detect samples and improve performance.As shown in Fig. 14, the negative value of LO2 is related to the lower value of the before curve (red) in comparison to the after curve (violet) of LO2 in Fig. 13.The LO2 cell line have been utilized as healthy cell measurements where the Herceptin and electrode couldn't detect it as the affinity of their binding site is lower.Thus, in binding or engagement cases, the cell presence increases the total resistance/impedance of the sensor.It may be related to the electronegativity of the LO2 cell line.

Sensitivity
The figure demonstrates how this gadget may linearly identify cancer cells.Since malignant cells are present in low concentration in real-life patient specimens (e.g., blood), the creation of a biosensor for real-time specimen analysis has produced an excellent result, with an R 2 = 0.996 in the range of 10 2 -10 6 cells (Figs. 15 and 16).

Stability
The measurement findings are significantly impacted by the degree of stability.For two weeks, the modified electrode was kept at room temperature to ensure verification.One indicator of the changed electrode's stability is the peak current of the voltammogram.According to the peak current, the amount is 97% of the starting value after one week and 92% of the beginning value after two weeks.Based on the findings, it can be concluded that the changed electrode would be reliable after two weeks.
Furthermore, the analyte is felt using the same process in each of these methods.As previously indicated, biosensing measurements were obtained using SWV, an effective technique.It is possible to conclude that the produced biosensor has superior sensitivity and stability by comparing the response characteristics of the produced biosensor for the detection of HER2 with the response characteristics of other rGO-based biosensors, such as Fe 3 O 4 and PANI-based biosensors published in the literature (Table 4).

Conclusion
Instead of using laborious and backbreaking techniques for early detection, scientists are now required by the medical business and expanding demand for clinical cancer research.To improve survival rates and quality of life, isolating cancer cells is just as crucial as detection.The creation of early-cancer diagnostic systems has been

Figure 1 .
Figure 1.Schematic process diagram for the fabrication and functionalization of sandwich rGO/Fe 3 O 4 /Nafion/ PANI for the detection of SK-BR3 cell line.

2 Figure 11 .
Figure 11.A 3D response surface of interaction between incubation time and nafion.

Figure 12 .
Figure 12.Predicted vs. actual values based on CCD.

Figure 13 .
Figure 13.Selectivity of the biosensor and the comparison of different cell lines on the sensing performance (a) SK-BR-3, (b) MCF-7, and (c) LO2.Red and violet curves are related to before and after depositing cells, respectively.

Figure 14 .
Figure 14.Effect of several cells on the electrode response and a comparison of the biosensor activity in the presence of the cells of MCF-7, SK-BR-3, and LO2.

Figure 15 .
Figure 15.SWV responses of our biosensor for detection of HER2 in different numbers of cells ranging from 10 2 to 10 6 cells.All tests were repeated at least 3 times (Temperature of 37 °C; pH 7.4).

Figure 16 .
Figure 16.Calibration curve for different numbers of SK-BR3 BC cells under optimal sensing conditions.These tests were performed in a solution containing 5 mM K 3 Fe(CN) 6 , 5 mM K 4 Fe(CN) 6 and 0.01 M PBS.Every measurement was repeated 3 times (n = 3).

Table 2 .
Design of experiments: factorial design and supplementary experiments of CCD.

Table 3 .
ANOVA for response surface quadratic model.

Table 4 .
Different electrochemical biosensors for tumor cell detection. S.